\documentclass[twocolumn,twoside]{article}
\makeatletter\if@twocolumn\PassOptionsToPackage{switch}{lineno}\else\fi\makeatother

\usepackage{amsfonts,amssymb,amsbsy,latexsym,amsmath,tabulary,graphicx,times,xcolor}

%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%
% Following additional macros are required to function some 
% functions which are not available in the class used.
%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%
\usepackage{url,multirow,morefloats,floatflt,cancel,tfrupee}
\makeatletter


\AtBeginDocument{\@ifpackageloaded{textcomp}{}{\usepackage{textcomp}}}
\makeatother
\usepackage{colortbl}
\usepackage{xcolor}
\usepackage{pifont}
\usepackage[nointegrals]{wasysym}
\urlstyle{rm}
\makeatletter

%%%For Table column width calculation.
\def\mcWidth#1{\csname TY@F#1\endcsname+\tabcolsep}

%%Hacking center and right align for table
\def\cAlignHack{\rightskip\@flushglue\leftskip\@flushglue\parindent\z@\parfillskip\z@skip}
\def\rAlignHack{\rightskip\z@skip\leftskip\@flushglue \parindent\z@\parfillskip\z@skip}

%Etal definition in references
\@ifundefined{etal}{\def\etal{\textit{et~al}}}{}


%\if@twocolumn\usepackage{dblfloatfix}\fi
\usepackage{ifxetex}
\ifxetex\else\if@twocolumn\@ifpackageloaded{stfloats}{}{\usepackage{dblfloatfix}}\fi\fi

\AtBeginDocument{
\expandafter\ifx\csname eqalign\endcsname\relax
\def\eqalign#1{\null\vcenter{\def\\{\cr}\openup\jot\m@th
  \ialign{\strut$\displaystyle{##}$\hfil&$\displaystyle{{}##}$\hfil
      \crcr#1\crcr}}\,}
\fi
}

%For fixing hardfail when unicode letters appear inside table with endfloat
\AtBeginDocument{%
  \@ifpackageloaded{endfloat}%
   {\renewcommand\efloat@iwrite[1]{\immediate\expandafter\protected@write\csname efloat@post#1\endcsname{}}}{\newif\ifefloat@tables}%
}%

\def\BreakURLText#1{\@tfor\brk@tempa:=#1\do{\brk@tempa\hskip0pt}}
\let\lt=<
\let\gt=>
\def\processVert{\ifmmode|\else\textbar\fi}
\let\processvert\processVert

\@ifundefined{subparagraph}{
\def\subparagraph{\@startsection{paragraph}{5}{2\parindent}{0ex plus 0.1ex minus 0.1ex}%
{0ex}{\normalfont\small\itshape}}%
}{}

% These are now gobbled, so won't appear in the PDF.
\newcommand\role[1]{\unskip}
\newcommand\aucollab[1]{\unskip}
  
\@ifundefined{tsGraphicsScaleX}{\gdef\tsGraphicsScaleX{1}}{}
\@ifundefined{tsGraphicsScaleY}{\gdef\tsGraphicsScaleY{.9}}{}
% To automatically resize figures to fit inside the text area
\def\checkGraphicsWidth{\ifdim\Gin@nat@width>\linewidth
	\tsGraphicsScaleX\linewidth\else\Gin@nat@width\fi}

\def\checkGraphicsHeight{\ifdim\Gin@nat@height>.9\textheight
	\tsGraphicsScaleY\textheight\else\Gin@nat@height\fi}

\def\fixFloatSize#1{}%\@ifundefined{processdelayedfloats}{\setbox0=\hbox{\includegraphics{#1}}\ifnum\wd0<\columnwidth\relax\renewenvironment{figure*}{\begin{figure}}{\end{figure}}\fi}{}}
\let\ts@includegraphics\includegraphics

\def\inlinegraphic[#1]#2{{\edef\@tempa{#1}\edef\baseline@shift{\ifx\@tempa\@empty0\else#1\fi}\edef\tempZ{\the\numexpr(\numexpr(\baseline@shift*\f@size/100))}\protect\raisebox{\tempZ pt}{\ts@includegraphics{#2}}}}

%\renewcommand{\includegraphics}[1]{\ts@includegraphics[width=\checkGraphicsWidth]{#1}}
\AtBeginDocument{\def\includegraphics{\@ifnextchar[{\ts@includegraphics}{\ts@includegraphics[width=\checkGraphicsWidth,height=\checkGraphicsHeight,keepaspectratio]}}}

\DeclareMathAlphabet{\mathpzc}{OT1}{pzc}{m}{it}

\def\URL#1#2{\@ifundefined{href}{#2}{\href{#1}{#2}}}

%%For url break
\def\UrlOrds{\do\*\do\-\do\~\do\'\do\"\do\-}%
\g@addto@macro{\UrlBreaks}{\UrlOrds}



\edef\fntEncoding{\f@encoding}
\def\EUoneEnc{EU1}
\makeatother
\def\floatpagefraction{0.8} 
\def\dblfloatpagefraction{0.8}
\def\style#1#2{#2}
\def\xxxguillemotleft{\fontencoding{T1}\selectfont\guillemotleft}
\def\xxxguillemotright{\fontencoding{T1}\selectfont\guillemotright}

\newif\ifmultipleabstract\multipleabstractfalse%
\newenvironment{typesetAbstractGroup}{}{}%

%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%%

\usepackage[authoryear]{natbib}



\newif\ifnokeywords\nokeywordsfalse

\makeatletter\input{size10-pointfive.clo}\makeatother%
\definecolor{kwdboxcolor}{RGB}{242,242,242}
\usepackage[hidelinks,colorlinks=true,allcolors=blue]{hyperref}
\linespread{1}                 
\def\floatpagefraction{0.8}

\usepackage[paperheight=11.69in,paperwidth=8.26in,top=1in,bottom=1in,left=1in,right=.75in,headsep=24pt]{geometry}

\usepackage{multirow-custom}

\makeatletter

\def\hlinewd#1{%
  \noalign{\ifnum0=`}\fi\hrule \@height #1%
  \futurelet\reserved@a\@xhline}
\def\tbltoprule{\hlinewd{1pt}\\[-14pt]}
\def\tblbottomrule{\noalign{\vspace*{6pt}}\hline\noalign{\vspace*{2pt}}}
\def\tblmidrule{\hline\noalign{\vspace*{2pt}}}



\let\@articleType\@empty
\let\@journalDoi\@empty
\let\@journalVolume\@empty
\let\@journalIssue\@empty
\let\@crossMarkLink\@empty
\let\@receivedDate\@empty
\let\@acceptedDate\@empty
\let\@revisedDate\@empty
\let\@publishedDate\@empty
\let\@copyrightYear\@empty
\let\@firstPage\@empty
\def\articleType#1{\gdef\@articleType{#1}}
\def\journalDoi#1{\gdef\@journalDoi{#1}}
\def\crossMarkLink#1{\gdef\@crossMarkLink{#1}}
\def\receivedDate#1{\gdef\@receivedDate{#1}}
\def\acceptedDate#1{\gdef\@acceptedDate{#1}}
\def\revisedDate#1{\gdef\@revisedDate{#1}}
\def\publishedDate#1{\gdef\@publishedDate{#1}}
\def\copyrightYear#1{\gdef\@copyrightYear{#1}}
\def\journalVolume#1{\gdef\@journalVolume{#1}}
\def\journalIssue#1{\gdef\@journalIssue{#1}}
\def\firstPage#1{\gdef\@firstPage{#1}}
\let\@issuelogo\@empty%
\let\@issuelogoex\@empty%
\def\issuelogo#1{\gdef\@issuelogo{#1}}
\def\issuelogoex#1{\gdef\@issuelogoex{#1}}


\def\author#1{%
  \gdef\@author{%
    \hskip-\dimexpr(\tabcolsep)\hskip5pt%
    \parbox{\dimexpr\textwidth-1pt}%
    {\fontsize{11}{13}\selectfont\raggedright #1}%
  }%
}


\usepackage{pharmascope-abs}
\usepackage{caption}
\usepackage{lastpage}
\usepackage{fancyhdr}
\usepackage[noindentafter,explicit]{titlesec}
\usepackage{fontspec}

\setmainfont[%
BoldFont=cambriab.ttf,%
ItalicFont=CAMBRIAI.TTF,%
BoldItalicFont=CAMBRIAZ.TTF]{Cambria.ttf}
\lefthyphenmin = 3

\def\title#1{%
  \gdef\@title{%
      \vspace*{-40pt}%
       \ifx\@articleType\@empty\else{\fontsize{10}{12}\scshape\selectfont\hspace{8pt}\@articleType\hfill\mbox{}\par\vspace{2pt}}\fi%
       \minipage{\linewidth}
         \hrulefill\\[-0.7pt]%%{\includegraphics[width=75pt,height=50pt]{ijrps_logo.png}}\hfill
         \mbox{~}\hspace{5pt}\parbox{.1\linewidth}{\IfFileExists{images/\@issuelogo.\@issuelogoex}{\includegraphics[width=79pt,height=61pt]{images/\@issuelogo.\@issuelogoex}}{\includegraphics[width=75pt,height=50pt]{ijrps_logo.png}}}\hfill
         \fcolorbox{kwdboxcolor}{kwdboxcolor}{\parbox{.792\linewidth}{%
          \begin{center}\fontsize{17}{17}\selectfont\scshape\vskip-7pt International Journal of Research in Pharmaceutical Sciences\hfill\end{center}%
          \vspace*{-10pt}\hspace*{4pt}{\fontsize{8}{9}\selectfont Published by JK Welfare \& Pharmascope Foundation\hfill  Journal Home Page: \href{www.ijrps.com}{\color{blue}\underline{\smash{www.ijrps.com}}}}\hspace*{4pt}\mbox{}}}%
       \par\vspace*{-1pt}\rule{\linewidth}{1.3pt}%
       \endminipage%
    \par\vspace*{9.2pt}\parbox{.98\linewidth}{\linespread{.9}\raggedright\fontsize{14}{17}\selectfont #1}%
    \vspace*{-8pt}%
  }
}


\setlength{\parindent}{0pt}
\setlength{\parskip}{0.4pc plus 1pt minus 1pt}

\def\abbrvJournalTitle{Int. J. Res. Pharm. Sci.}

\fancypagestyle{headings}{%
  \renewcommand{\headrulewidth}{0pt}%
  \renewcommand{\footrulewidth}{0.3pt}
  \fancyhf{}%
  \fancyhead[R]{%
    \fontsize{9.12}{11}\selectfont\RunningAuthor,\ \abbrvJournalTitle,\ \ifx\@journalVolume\@empty X\else\@journalVolume\fi%
    \ifx\@journalIssue\@empty\else(\@journalIssue)\fi%
    ,\ \ifx\@firstPage\@empty 1\else\@firstPage\fi-\pageref*{LastPage}%
  }%
  \fancyfoot[LO,RE]{\fontsize{9.12}{11}\selectfont\textcopyright\ International Journal of Research in Pharmaceutical Sciences}%
  \fancyfoot[RO,LE]{\fontsize{9.12}{11}\selectfont\thepage}
}\pagestyle{headings}

                                                         
\fancypagestyle{plain}{%
  \renewcommand{\headrulewidth}{0pt}%
  \renewcommand{\footrulewidth}{0.3pt}%
  \fancyhf{}%
  \fancyhead[R]{%
    \fontsize{9.12}{11}\selectfont\RunningAuthor,\ \abbrvJournalTitle,\ \ifx\@journalVolume\@empty X\else\@journalVolume\fi%
    \ifx\@journalIssue\@empty\else(\@journalIssue)\fi%
    ,\ \ifx\@firstPage\@empty 1\else\@firstPage\fi-\pageref*{LastPage}%
  }%
  \fancyfoot[LO,RE]{\fontsize{9.12}{11}\selectfont\textcopyright\ International Journal of Research in Pharmaceutical Sciences}%
  \fancyfoot[RO,LE]{\fontsize{9.12}{11}\selectfont\thepage}
  \ifx\@firstPage\@empty\else\setcounter{page}{\@firstPage}\fi
}


\def\NormalBaseline{\def\baselinestretch{1.1}}
\usepackage{textcase}
\setcounter{secnumdepth}{0}

\titleformat{\section}[block]{\bfseries\boldmath\NormalBaseline\filright\fontsize{10.5}{13}\selectfont}
{\thesection}
{6pt}
{\MakeTextUppercase{#1}}
[]
\titleformat{\subsection}[block]{\bfseries\boldmath\NormalBaseline\filright\fontsize{10.5}{12}\selectfont}
{\thesubsection}
{6pt}
{#1}
[]
\titleformat{\subsubsection}[block]{\NormalBaseline\filright\fontsize{10.5}{12}\selectfont}
{\thesubsubsection}
{6pt}
{#1}
[]
\titleformat{\paragraph}[block]{\NormalBaseline\filright\fontsize{10.5}{10}\selectfont}
{\theparagraph}
{6pt}
{#1}
[]
\titleformat{\subparagraph}[block]{\NormalBaseline\filright\fontsize{10.5}{12}\selectfont}
{\thesubparagraph}
{6pt}
{#1}
[]

\titlespacing{\section}{0pt}{.5\baselineskip}{.5\baselineskip}  
\titlespacing{\subsection}{0pt}{.5\baselineskip}{.5\baselineskip}  
\titlespacing{\subsubsection}{0pt}{.5\baselineskip}{.5\baselineskip}  
\titlespacing{\paragraph}{0pt}{.5\baselineskip}{.5\baselineskip}  
\titlespacing{\subparagraph}{0pt}{.5\baselineskip}{.5\baselineskip}

\captionsetup[figure]{skip=1.4pt,font=bf,labelsep=colon,justification=raggedright,singlelinecheck=false}
\captionsetup[table]{skip=1.4pt,font=bf,labelsep=colon,justification=raggedright,singlelinecheck=false}

\def\bibyear#1{#1}
%\def\bibjtitle#1{#1}   %%Publisher request
\def\bibauand{}
\setlength\bibsep{3pt}
\setlength\bibhang{8pt}

\makeatother
\date{}


\usepackage[flushleft]{threeparttablex}

\usepackage{float}

\begin{document}


\def\RunningAuthor{Shivkanya Fuloria et al.}
\firstPage{1849}
\articleType{Original Article}
\receivedDate{03 Jan 2020}
\acceptedDate{17 Jan 2020}
\revisedDate{15 Jan 2020}
\journalVolume{2020, 11}
\journalIssue{2}
\journalDoi{ijrps.v11i2.2092}
\copyrightYear{2020}
\def\authorCount{8}
\def\affCount{1}

\def\journalTitle{International Journal of Research in Pharmaceutical Sciences}

\title{\textbf{Biosynthesis of DLLAE blended silver nanoparticles and their response against periodontitis triggering bacteria} \textbf{\space }}
\author{Chin~Zi~Hang,  
            Neeraj~Kumar~Fuloria,  
            Oh~Jian~Hong,  
            Chuah~Bee~Kim,  
            Bernice~Yii~Shu~Ting,  
            Chiam~Sin~Ru,  
            Mok~Yong~Ko, 
            Shivkanya~Fuloria\textsuperscript{*}~\\[5pt]{Faculty of Pharmacy, AIMST University, Kedah - 08100, Malaysia}}

\begin{abstract}
Facts over microorganisms to predominate periodontitis, shifting of human microbiota by \textit{Dimocarpus longan (D. longan) }plant\textit{,} and potentiation of antimicrobial activity by biosynthetic silver nanoparticles (SNPs) intended present study to biosynthesize, optimize, characterize and evaluate the antimicrobial potential of silver nanoparticles (SNPs) obtained using \textit{D. longan} leaves aqueous extract (DLLAE). Study involved preparation of DLLAE using decoction method. The DLLAE was subjected to biosynthesis of SNPs followed by optimization (using UV-Visible spectrometry), characterization (by FTIR, FESEM, XRD, and EDX), stability, and antimicrobial activity of SNPs against periodontitis triggering human microflora. Biosynthesized SNPs exhibited signal between 416-453 nm. Optimization study established AgNO\ensuremath{_{3}} concentration (5 mM), pH 4, DLLAE and AgNO\ensuremath{_{3\ }} ratio (1:9) and temperature (60\ensuremath{^\circ}C) as parametric requirement for SNPs biosynthesis using DLLAE. Stability study exhibited signal between 489-553 nm supporting SNPs stability. Characterization data of FESEM showed that SNPs were poly dispersed, and spherical shaped. Biosynthesized SNPs size ranged from 74.82 nm to 131.5 nm. The XRD data revealed presence of signals at 38.08\ensuremath{^\circ}, 44.33\ensuremath{^\circ}, 64.47\ensuremath{^\circ}, and 78.83\ensuremath{^\circ} 2\ensuremath{\theta } values indexed to silver cubic structure planes. In EDX study, silver exhibited strong signal (55.54\%). Antimicrobial investigation explored the high inhibitory potential of SNPs against \textit{B. subtilis and P. aeruginosa} and low inhibitory potential against \textit{S. aureus}\textit{ and E. coli}.  Present study conclude that biosynthesis of SNPs using DLLAE is an efficient method and biosynthetic SNPs possess high antimicrobial potential against \textit{P. aeruginosa } \textit{and B. subtilis} the periodontitis triggering pathogens.
\end{abstract}\def\keywordstitle{Keywords}

\begin{keywords}SNPs,\newline D. Longan,\newline Optimization,\newline Characterization,\newline Antimicrobial
\end{keywords}
\twocolumn[ \maketitle {\printKwdAbsBox}]
\makeatletter{\raggedright\textsuperscript{*}Corresponding Author\par Name:\ Shivkanya~Fuloria~\\ Phone:\ +604429800~\\  Email:\ shivani2jaju@gmail.com
        \par}\vspace*{-11pt}\hrulefill\par{\fontsize{12}{14}\selectfont ISSN: 0975-7538}\par% 
        \textsc{DOI:}\ \href{https://doi.org/10.26452/\@journalDoi}{\textcolor{blue}{\underline{\smash{https://doi.org/10.26452/\@journalDoi}}}}\par%
        \vspace*{-11pt}\hrulefill\\{\fontsize{9.12}{10.12}\selectfont Production and Hosted by}\par{IJRPS |~\href{www.ijrps.com}{www.ijrps.com}}\par%
        \vspace*{-2pt}{\fontsize{9.12}{10.12}\selectfont\textcopyright\ \@copyrightYear\ $|$ All rights reserved.}\par%
        \vspace*{-11pt}\rule{\linewidth}{1.2pt}
        \makeatother
        
    
\section{Introduction}
Current decade reports humans to own 1:1 bacteria and cells. A small disturbance in human microbiota manifests in several infectious diseases \unskip~\citep{692917:16400318}. Among all infectious disease periodontitis is claimed to be most complicated microbial infection. Periodontitis is connected with dental biofilm dysbiosis, which results in chronic inflammation of soft tissue periodontal lining, and tooth/alveolar bone destruction \unskip~\citep{692917:16399997}. Periodontitis manifests in progression of cancer, cardiovascular diseases, obesity, respiratory disease, rheumatoid arthritis, and diabetes. Facts suggest \textit{Pseudomonas aeruginosa (P. aeruginosa), Staphylococcus aureus (S. aureus)}, \textit{Escherichia coli (E. coli), }and \textit{Bacillus subtilis (B. subtilis) }to trigger periodontitis. Several conventional antimicrobials used in periodontitis infections offers adverse effects like multiple drug resistance, immune suppression, allergic reactions, and high mortality risk. Thus, there is a necessity for natural alternatives \unskip~\citep{692917:16399870}.\textbf{\space }

Current decade witnesses enormous research over SNPs ability to augment the antimicrobials and other biomedicines activity. The inherent properties (like: high antibiotic potential, increased shelf life, low toxicity, cost-effectiveness, and easy availability of herbal drugs) always challenges the researchers to investigate drugs for treatment of periodontal infections using plants source \unskip~\citep{692917:16399955}. Formulation of SNPs using \textit{D. longan} seeds extracts (bearing high antimicrobial activity) attracts the investigators \unskip~\citep{692917:16400081}, but formulation of SNPs using \textit{D. longan} leaves is yet an area to be explored. Based on the evidences, current study was planned to biosynthesize CSNPS using DLLAE and evaluate against periodontitis triggering bacteria.\textit{\textbf{\space }}
    
\section{Materials and Methods}
The chemicals like: potassium bromide (KBr), silver nitrate (AgNO\ensuremath{_{3}}), sodium hydroxide (NaOH), calcium chloride (CaCl\ensuremath{_{2}}), sodium oxalate, sodium chloride, Tris buffer,  dimethyl sulfoxide (DMSO), and nutrient agar were procured from Fisher chemicals, Sigma Aldrich, SD Fine, and Hi-Media. The SNPs were biosynthesized using \textit{Dimocarpus longan} leaves aqueous extract (DLLAE). The glass wares were cleaned using (deionized water), dried (at 160\ensuremath{^\circ}C) and plastic ware were autoclaved before initiation of antimicrobial experiment. 

\textbf{DLLAE preparation}

The experimental procedure for DLLAE preparation was based on reported method with slight modification \unskip~\citep{692917:16399841}. Briefly, the fresh \textit{D. longan} leaves were collected (from Kampung Baru, Bedong, Kedah, Malaysia), washed with water (for impurities elimination), dried (40-50\ensuremath{^{o}}C), and powdered (using blender) for further investigation. The \textit{D. longan} leaves aqueous extract (DLLAE) was prepared by boiling mixture of blended \textit{D. longan} leaves powder (25 g), de-ionised water (95 ml) and ethanol (5 ml). Mixture was allowed to cool and filtered using 4-fold muslin cloth and Whatman no. 1 filter paper to offer pure DLLAE. The DLLAE which was stored at 8-10\ensuremath{^\circ}C in a refrigerator subjected to further investigations and SNPs synthesis.

\textbf{SNPs biosynthesis}

The biosynthesis of SNPs was conducted according to the reported procedure with slight modification \unskip~\citep{692917:16399870,692917:16399955}. Briefly, the SNPs biosynthesis was done by mixing 1 ml of \textit{D. longan} extract with 9 ml of AgNO\ensuremath{_{3}}\ensuremath{_{}}solution (5 mM). The mixture was left for incubation for 24 h in a dark cardboard to undergo reduction. The AgNO\ensuremath{_{3\ }}solution after reduction (change in color to brown), was subjected to centrifugation for 90 minutes at 5000 rpm. 

Supernatant layer was removed off to yield SNPs. The SNPs were further rewashed with deionized water, re-centrifuged (using the same parameters) and air dried to yield pure SNPs. This process of rewashing was repeated 2 to 3 times to remove the unwanted substance over SNPs surface).

\textbf{UV-Visible Analysis}

The SNPs biosynthesis was determined using UV{\textendash}Visible spectrometry. In 10 ml volumetric flask, 1 mg of dried SNPs was dissolved in 10 ml deionized water. Test mixture was analyzed by UV{\textendash}Visible spectrometer at 200 to 800 nm to detect the surface plasmon resonance (SPR) peak. 

\textbf{Optimization of parameters for SNPs biosynthesis }

The SNPs biosynthesis was optimized based on UV-Visible spectrometric studies over DLLAE and AgNO\ensuremath{_{3\ }}reaction mixture, maintained under different parametric conditions, such as: AgNO\ensuremath{_{3\ }}concentration, DLLAE and AgNO\ensuremath{_{3\ }}ratio, pH and temperature. The optimization of SNPs was conducted as per reported protocols with minor modifications \unskip~\citep{692917:16399870}. 

All the reaction mixtures were visually examined (for color change) and subjected to UV-Visible spectrometry (to observe the SPR signal) after 24 h of incubation maintaining same reaction conditions except for individual parameters.

\textbf{Optimization of AgNO\ensuremath{_{3}} concentration }

To optimize the biosynthesis of SNP based on AgNO\ensuremath{_{3}} concentration, the SNPs biosynthesis involved preparation of five individual reaction mixtures with difference in AgNO\ensuremath{_{3}} concentration, such as: 1, 2, 3, 4, and 5 mM.  

\textbf{Optimization of volumetric ratio of DLLAE to AgNO\ensuremath{_{3}}}

To optimize the biosynthesis of SNP based on DLLAE and AgNO\ensuremath{_{3}} ratio, the SNPs biosynthesis involved preparation of nine individual reaction mixtures in nine different ratios of DLLAE and AgNO\ensuremath{_{3,}} such as: 1:9, 2:8, 3:7, 4:6, 5:5, 6:4, 7:3, 8:2 and 9:1.  

\textbf{Optimization of temperature}

To optimize the biosynthesis of SNP based on temperature, the SNPs biosynthesis involved preparation of three individual reaction mixtures with difference in temperatures, such as: 4\ensuremath{^\circ}C, 25\ensuremath{^\circ}C room temperature and 60\ensuremath{^\circ}C. 

\textbf{Optimization of } \textbf{pH}

To biosynthesized SNPs were optimized based on pH, the SNPs biosynthesis involved preparation of four individual reaction mixtures with difference in pH, such as pH 4, pH 5, pH 7 and pH 8. The reaction mixtures pH was adjusted using 0.1 N NaOH and 0.1 N HCl.\textbf{\space }

\textbf{Stability study of biosynthesized SNPs }

The stability of biosynthesized SNPs was determined on the basis of SPR signal range (340 to 540 nm). The readings were taken on 0 h, \ensuremath{\frac12}  h, 2 h, 24 h, 7 d and 15 d intervals.  

\textbf{SNPs characterization}

The biosynthesized SNPs were characterized based on other standard research studies \unskip~\citep{692917:16399998}. Before characterization, the synthesized SNPs were subjected to purification. This was done to avoid interaction of extract absorbance with nanoparticles absorbance. The characterization of SNPs was done using Fourier transformed infrared spectrometer (FT-IR), X-ray diffraction (XRD), Energy-dispersive X-ray (EDX) analysis instrument and field emission scanning electron microscope (FESEM). The formation of biosynthesized SNPs was determined based on a change in color of the solution, UV{\textendash}Visible spectrometer (Shimadzu U-2800) and FT-IR (PerkinElmer SLE/MSC4/29) spectral data. The FESEM measurement was performed to understand the morphology of SNPs. The SNPs crystal nature was examined by X-Ray diffractometer. The EDX analysis was performed by FEI Nova Nano SEM 450 with EDX assembly.  


\bgroup
\fixFloatSize{images/95a8c5f7-b4d8-429d-b4ba-e27850b70745-upicture1.png}
\begin{figure}[!htbp]
\centering \makeatletter\IfFileExists{images/95a8c5f7-b4d8-429d-b4ba-e27850b70745-upicture1.png}{\includegraphics{images/95a8c5f7-b4d8-429d-b4ba-e27850b70745-upicture1.png}}{}
\makeatother 
\caption{\boldmath {Colour changes from yellowish-brown to brown}}
\label{f-501aa3c0d08d}
\end{figure}
\egroup
\textbf{Antimicrobial activity of biosynthesized SNPs}

The experimental method was based on other investigation studies with minor developments \unskip~\citep{692917:16400314}. The biosynthetic SNPs were evaluated for antimicrobial potential against \textit{P. aeruginosa} (ATCC 25619), \textit{B. subtilis} (ATCC 6633), \textit{S. aureus} (ATCC 29737) and \textit{E. coli} (ATCC 8739) by well diffusion technique. The fresh and pure culture of each bacterial strain was sub cultured over nutrient broth (NB) at 37\ensuremath{^\circ}C (previously shaken on a rotary shaker at 130 rpm). The culture of each bacteria was swabbed over nutrient agar plates. The wells of 8 mm size were drilled over nutrient agar plates. In each well of nutrient agar plate, using micropipette were added DLLAE (10, 20, 40, 60, 80 and 100 \ensuremath{\mu}g/mL), SNPs (10, 20, 40, 60, 80 and 100 \ensuremath{\mu}g/mL), and ciprofloxacin (50 \ensuremath{\mu}g/mL) each in with 50 \ensuremath{\mu}l volume. The inhibitory zones were measured after incubating the plates for 24 h at 37\ensuremath{^\circ}C.  
    
\section{Results and Discussion}
The SNPs biosynthesis was assessed visually and through UV-Visible analysis. The stirred mixture of AgNO\ensuremath{_{3}} solution and DLLAE was kept aside for 24 h at room temperature to monitor the color change. The solution color change to brown revealed the Ag\ensuremath{^{+}} reduction (Figure~\ref{f-501aa3c0d08d}). The current study data established the successful biosynthesis of SNPs using DLLAE. Biosynthesis of SNPs occurred, when AgNO\ensuremath{_{3}} was exposed to DLLAE. Visual examination of color change confirmed the SNPs biosynthesis and Ag\ensuremath{^{+}} reduction. The color change was attributed to surface plasmon resonance property, conceivably a result of stimulation of longitudinal plasmon vibrations stimulation \unskip~\citep{692917:16399998,692917:16399870}.


\bgroup
\fixFloatSize{images/c1a72da1-1c44-4d97-88a6-aa9646182182-upicture2.png}
\begin{figure*}[!htbp]
\centering \makeatletter\IfFileExists{images/c1a72da1-1c44-4d97-88a6-aa9646182182-upicture2.png}{\includegraphics{images/c1a72da1-1c44-4d97-88a6-aa9646182182-upicture2.png}}{}
\makeatother 
\caption{\boldmath {Optimization of AgNO\ensuremath{_{3}} (2A), Optimization of volumetric ratio of DLLAE ratio to AgNO\ensuremath{_{3}} (2B), Optimization of temperature (2C), Optimization of pH (2D)}}
\label{f-5be1e22740b6}
\end{figure*}
\egroup
\textbf{Optimization of parameters for SNPs biosynthesis reaction mixture }

The optimization of parameters for SNPs biosynthesis reaction mixture was founded on: AgNO\ensuremath{_{3}} concentration, DLLAE and AgNO\ensuremath{_{3}} ratio, temperature and pH\textit{.} In present investigation, the optimization data was validated based on SPR range of standard investigations \unskip~\citep{692917:16399869} \textit{. }

\textbf{Optimization of AgNO\ensuremath{_{3\ }}concentration}

The biosynthesized SNPs optimization based on five concentrations of AgNO\ensuremath{_{3}} (1, 2, 3, 4 and 5 mM) as parameter offered a UV-Vis. plot comprising five curves (Curve 1, 2, 3, 4 and 5) shown in Figure~\ref{f-5be1e22740b6}(A). The UV-visble spectrum exhibited the curves at 447 nm (1 mM), 445 nm (2 mM), 449 nm (3mM), 449 nm (4mM) and 450 nm (5mM). A shifting in SPR signal was observed on increasing the AgNO\ensuremath{_{3\ }}concentration. 

The spectrum in Figure~\ref{f-5be1e22740b6}(A), revealed maximum absorption for 5 mM of silver nitrate solution (450 nm). Hence, 5 mM of AgNO\ensuremath{_{3\ }}concentration was considered as optimum for biosynthesis of SNPs. Optimization data for AgNO\ensuremath{_{3}} was also supported by SPR signal range of other research \unskip~\citep{692917:16399841}. 


\bgroup
\fixFloatSize{images/d7aea7df-77ee-46a3-87f5-ac8492877c59-upicture3.png}
\begin{figure}[!htbp]
\centering \makeatletter\IfFileExists{images/d7aea7df-77ee-46a3-87f5-ac8492877c59-upicture3.png}{\includegraphics{images/d7aea7df-77ee-46a3-87f5-ac8492877c59-upicture3.png}}{}
\makeatother 
\caption{\boldmath {Stability study of bio synthesized SNPs}}
\label{f-8269346445e8}
\end{figure}
\egroup
\textbf{Optimization of volumetric ratios of DLLAE and AgNO\ensuremath{_{3}}}

The biosynthesized SNPs optimization based on nine ratios of DLLAE and AgNO\ensuremath{_{3}} (1:9, 2:8, 3:7, 4:6, 5:5, 6:4, 7:3, 8:2 and 9:1) as parameter offered a UV-Vis. plot comprising nine curves (Curve 1, 2, 3, 4, 5, 6, 7, 8 and 9) shown in Figure~\ref{f-5be1e22740b6}(B). Curve 1 represented the absorbance peak at 418 nm, which confirmed with the formation of SNPs. The other curves showed the absorbance peaks within the range of 650 nm to 656 nm, which were not fall within the range of SNPs formation. Therefore, the volumetic ratio of DLLAE to AgNO\ensuremath{_{3\ }}(1:9) was considered as optimum for biosynthesis of SNPs. The optimization study results for volumetric ratio of DLLAE and AgNO\ensuremath{_{3\ }}(1:9) were also supported by the SPR signal range of other research studies \unskip~\citep{692917:16399955,692917:16399869}\textit{.}

\textbf{Optimization of temperature}

The biosynthesized SNPs optimization based on temperature (4\ensuremath{^\circ}C, 25\ensuremath{^\circ}C and 60\ensuremath{^\circ}C) as parameter offered a UV-Vis. plot comprising three curves (Curve 1, 2, and 3) shown in Figure~\ref{f-5be1e22740b6}(C). The UV-Visible spectrum, showed the effect of temperature on the synthesis of SNPs. The Figure~\ref{f-5be1e22740b6}(C) UV-Visible spectrum, exhibited no SNPs signals in curve 1 and 2 (4\ensuremath{^\circ}C and 25\ensuremath{^\circ}C). The spectrum exhibited SNPs signal in curve 3 (60\ensuremath{^\circ}C) at 453 nm revealing the completion of SNPs synthesis. The absorption spectrum (Figure~\ref{f-5be1e22740b6}C) revealed that, room temperature and 4\ensuremath{^\circ}C (representing curve 2 and 1) were not ideal to formulate SNPs. Whereas, 60\ensuremath{^\circ}C (representing curve 3) was the ideal temperature to produce SNPs displaying signal at 453 nm. Hence, maintaining the reaction at 60\ensuremath{^\circ}C was considered as optimum for SNPs biosynthesis. The results of optimization study over SNPs biosynthesis were also supported by other literary evidences \unskip~\citep{692917:16400315,692917:16399869}\textit{.}

\textbf{Optimization of SNPs synthesis reaction mixture for pH}

The optimization of SNPs synthesis based on four pH (pH 4, pH 5, pH 7 and pH 8) yielded a spectrum in Figure~\ref{f-5be1e22740b6}(D), comprising four curves 1, 2, 3 and 4. UV-Visible spectrum, exhibited no signals for SNPs in curve 2, 3 and 4 (pH 8, pH 7 and pH 5). The spectrum displayed an SPR peak for SNPs in curve 1 (pH 4) at 416 nm revealing the SNPs synthesis. The Figure~\ref{f-5be1e22740b6}(D) UV-Visible spectrum produced on analysis of SNPs biosynthetic reaction at pH (4, 5, 7 and 8) revealed that pH 8, pH 7 and pH 5 (representing curve 2,3 and 4) were unsuitable to formulate SNPs. Whereas, pH 4 (representing curve 1) was ideal to produce SNPs displaying signal at 416 nm. Hence, maintaining the reaction at pH 4 was considered as optimum for SNPs biosynthesis. The pH optimization results for SNPs biosynthesis were supported by SPR signal range of other studies \unskip~\citep{692917:16400315,692917:16399869}\textit{.}

\textbf{Stability study for biosynthesized SNPs }

The stability study of biosynthesized SNPs using\textbf{\space }UV-Visible spectrometry experiment was conducted for 0 h, \ensuremath{\frac12}  h, 2 h, 24 h, 7 d and 15 d respectively. The results of stability study after fixing time as revealed that SPR signal was retained in the expected range.

The Figure~\ref{f-8269346445e8} illustrated of SNPs signal between 489 to 553 nm. It was observed that the spectra absorbance of SNPs was constant. Hence, s\textit{tability studies }showed that the SNPs were stable after 15 d. The present study SNPs signal range was also supported by other research studies \unskip~\citep{692917:16400315,692917:16399869}.


\bgroup
\fixFloatSize{images/aebbe49d-70d6-4253-968a-5844c94d08a3-upicture4.png}
\begin{figure*}[!htbp]
\centering \makeatletter\IfFileExists{images/aebbe49d-70d6-4253-968a-5844c94d08a3-upicture4.png}{\includegraphics{images/aebbe49d-70d6-4253-968a-5844c94d08a3-upicture4.png}}{}
\makeatother 
\caption{\boldmath {FTIR spectrum of pure DLLAE (A) and } biosynthesized SNPs (B)}
\label{f-40a59191f236}
\end{figure*}
\egroup

\bgroup
\fixFloatSize{images/77e581f5-376a-4645-8768-692c8fa0dcfa-upicture5.png}
\begin{figure*}[!htbp]
\centering \makeatletter\IfFileExists{images/77e581f5-376a-4645-8768-692c8fa0dcfa-upicture5.png}{\includegraphics{images/77e581f5-376a-4645-8768-692c8fa0dcfa-upicture5.png}}{}
\makeatother 
\caption{\boldmath {FESEM image of SNPs}}
\label{f-88dc42698d96}
\end{figure*}
\egroup

\bgroup
\fixFloatSize{images/4ad8ef30-afb2-4387-92cf-eae677a3c65e-upicture6.png}
\begin{figure*}[!htbp]
\centering \makeatletter\IfFileExists{images/4ad8ef30-afb2-4387-92cf-eae677a3c65e-upicture6.png}{\includegraphics{images/4ad8ef30-afb2-4387-92cf-eae677a3c65e-upicture6.png}}{}
\makeatother 
\caption{\boldmath {XRD image of SNPs}}
\label{f-e1b20443a734}
\end{figure*}
\egroup

\bgroup
\fixFloatSize{images/d5d308be-85a6-45d3-bad4-73680645002a-upicture7.png}
\begin{figure*}[!htbp]
\centering \makeatletter\IfFileExists{images/d5d308be-85a6-45d3-bad4-73680645002a-upicture7.png}{\includegraphics{images/d5d308be-85a6-45d3-bad4-73680645002a-upicture7.png}}{}
\makeatother 
\caption{\boldmath {EDX image of SNPs}}
\label{f-55b0f8ad4e0f}
\end{figure*}
\egroup

\begin{table*}[!htbp]
\caption{\boldmath {Zone of inhibition (in mm)} }
\label{tw-f47775a0ca97}
\centering 
\begin{threeparttable}

\def\arraystretch{1.1}
\ignorespaces 
\centering 
\begin{tabulary}{\linewidth}{p{\dimexpr.0799\linewidth-2\tabcolsep}p{\dimexpr.0591\linewidth-2\tabcolsep}p{\dimexpr.071\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.07\linewidth-2\tabcolsep}p{\dimexpr.09\linewidth-2\tabcolsep}}
\tbltoprule \rowcolor{kwdboxcolor}Microorganism & \multicolumn{13}{p{\dimexpr(.9200999999999999\linewidth-2\tabcolsep)}}{\cAlignHack Zone of Inhibition in mm}\\
\rowcolor{kwdboxcolor} & \multicolumn{6}{p{\dimexpr(.4101\linewidth-2\tabcolsep)}}{\cAlignHack SNPs} & \multicolumn{6}{p{\dimexpr(.42\linewidth-2\tabcolsep)}}{\cAlignHack D. longan Extract} & \cAlignHack Ciprofloxacin\\
\rowcolor{kwdboxcolor}Concentration (\ensuremath{\mu }g/ml) & \cAlignHack 10 & \cAlignHack 20 & \cAlignHack 40 & \cAlignHack 60 & \cAlignHack 80 & \cAlignHack 100 & \cAlignHack 10 & \cAlignHack 20 & \cAlignHack 40 & \cAlignHack 60 & \cAlignHack 80 & \cAlignHack 100 & \cAlignHack 50\\
\tblmidrule 
B. subtilis  &
  \cAlignHack 18 &
  \cAlignHack 18 &
  \cAlignHack 18 &
  \cAlignHack 24 &
  \cAlignHack 23 &
  \cAlignHack 25 &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack 21\\
S. aureus  &
  \cAlignHack 13 &
  \cAlignHack 14 &
  \cAlignHack 13 &
  \cAlignHack 15 &
  \cAlignHack 15 &
  \cAlignHack 14 &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack 21\\
P. aeruginosa &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack 20 &
  \cAlignHack 22 &
  \cAlignHack 23 &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack 21\\
E. coli  &
  \cAlignHack 14 &
  \cAlignHack 14 &
  \cAlignHack 14 &
  \cAlignHack 15 &
  \cAlignHack 15 &
  \cAlignHack 16 &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack N/A &
  \cAlignHack 20\\
\tblbottomrule 
\end{tabulary}\par 
\begin{tablenotes}\footnotesize 
    
\item{N/A: No activity}
\end{tablenotes}
\end{threeparttable}

\end{table*}
\textbf{Characterization of biosynthesized SNPs }

\textbf{Fourier Transformed Infrared (FTIR) analysis }

FTIR spectroscopy is used to identify the characteristic functional groups of chemical moieties. The FTIR experiment over the DLLAE and SNPs offered the two spectra given in Figure~\ref{f-40a59191f236}(A) and Figure~\ref{f-40a59191f236}(B). 

FTIR experiment determined the Ag\ensuremath{^{+ }}to Ag\ensuremath{^{0 }}reduction and SNPs synthesis. The DLLAE FTIR spectrum given in Figure~\ref{f-40a59191f236}(A) exhibited characteristic bands: 3466, 2891, 1693 cm\ensuremath{^{-1}}, attributed to O-H, C-H and C=O cm\ensuremath{^{-1}}vibrations respectively. IR spectrum of SNPs given in Figure~\ref{f-40a59191f236}(B), exhibited shifted and broadened IR bands at 3467, 2909, 1722, and 1541 cm\ensuremath{^{-1 }}attributed to O-H, C-H, C=O, C=N vibrations. 

The FTIR data revealed SNPs formation and Ag\ensuremath{^{+}} to Ag\ensuremath{^{0 }}reduction of \unskip~\citep{692917:16399870}. Based on comparison of FTIR spectra of DLLAE and biosynthesized\textbf{\space }SNPs, the DLLAE was recognized as dual capping (stabilizing) and reducing agent. The Figure~\ref{f-40a59191f236}(B) IR spectrum of SNPs was similar to figure IR spectrum of DLLAE, as it preserved majority of signals with marginal shifting and broadening. For example, 3466 cm\ensuremath{^{-1 }}(O-H vibrations) narrow band in Figure~\ref{f-40a59191f236}(A) FTIR spectrum of DLLAE was shifted to 3467 cm\ensuremath{^{-1 }}as a broad band in Figure~\ref{f-40a59191f236}(B) FTIR spectrum of SNPs \unskip~\citep{692917:16399869}

\textbf{Field Emission Scanning Electron Microscopy (FESEM)}

FESEM analysis is used to study the morphology of the biosynthetic SNPs \unskip~\citep{692917:16400082}. FESEM micrographs of SNPs are shown in Figure~\ref{f-88dc42698d96} with different magnifications. FESEM images showed that SNPs formed were polydispersed, spherical shaped. Particle sizes for SNPs ranged from 74.82 nm to 131.5 nm and were resulted by silver reduction by DLLAE from AgNO\ensuremath{_{3}}. 

\textbf{X-Ray diffraction (XRD) analysis}

The SNPs crystalline nature was analyzed by XRD pattern given in Figure~\ref{f-e1b20443a734}. The diffraction peaks at 2\ensuremath{\theta } values of 78.83, 64.47, 44.33, and 38.08 degrees can be indexed to face centered cubic structure of the silver reflection planes of SNPs. Apart from Bragg signals of silver nanocrystals, additional signals were also observed. These signals occur due to presence of biomolecules that are present in DLLAE. XRD results of SNPs were also verified by other studies \unskip~\citep{692917:16400316}. Average size of SNPs was determined to be 48.23 to 59. 06 nm using Debye{\textendash}Scherrer formula \unskip~\citep{692917:16400317}.

\textbf{Energy dispersive X-Ray diffraction (EDX) analysis}

EDX was used for elemental analysis to understand the presence of element involved in the SNPs development (Figure~\ref{f-55b0f8ad4e0f}). EDX data revealed strong signal for silver and confirmed the SNPs formation. The silver (55.54\%) was found as major element in comparison to carbon (21.16\%), oxygen (14.72 \%), and chlorine (3.84 \%). Usually, SNPs exhibits signal at 3 KeV attributed to SPR. The EDX data exhibited strong signal for silver and weak signal for oxygen, that may be due attributed to biomolecules bounded to SNPs surface \unskip~\citep{692917:16399842}.

\textbf{Antimicrobial activity of SNPs }

The SNPs are extensively used being antimicrobial and registered as more potent in comparison to silver ions. As per standard protocol \unskip~\citep{692917:16399955} the biosynthesized\textbf{\space }SNPs were investigated for their inhibition activity against \textit{S. aureus}, \textit{E. coli, P. aeruginosa}\textit{\space } and \textit{B.} \textit{subtilis.} The zone of inhibition (ZOI) was observed for each plate and the diameter was measured in mm (data given in Table~\ref{tw-f47775a0ca97}). The resultant data revealed that DLLAE possess no antimicrobial potential but when the same DLLAE was blended into SNPs, the SNPs of the same exhibited very strong antimicrobial potential.

The biosynthesized\textbf{\space }SNPs displayed highest zone of inhibition against \textit{B. subtilis } (25 mm) in 100 \ensuremath{\mu}g/mL dose. The pure DLLAE displayed no zone of inhibition against \textit{B. subtilis, E. coli, P. aeruginosa} and\textit{ S. aureus }(data given inTable~\ref{tw-f47775a0ca97}). When compared to ciprofloxacin, the SNPs exhibited a highest inhibition zone against \textit{B. subtilis, P. aeruginosa, E. coli,} and \textit{S. aureus} that is 25, 23, 16, and 14 mm respectively at 100 \ensuremath{\mu}g/mL dose. Interestingly, a pattern was observed in the antimicrobial activity of newer SNPs, when the concentration of SNPs was increased from 10 \ensuremath{\mu}g/mL to 100 \ensuremath{\mu}g/mL there was substantial rise in zone of inhibition. The antimicrobial activity results indicated that capping of silver with biochemical moieties of DLLAE (sugars, proteins, steroids, anthraquinones and coumarins glycosides, flavonoids, alkaloids, organic acid, tannic and phenolic compounds) caused a marked increase in the antimicrobial potential of SNPs formulated from DLLAE. This pattern of increment in antimicrobial response due to biochemical moieties is also supported by other investigations \unskip~\citep{692917:16399870}. Hence with it can be hypothesized that small sized SNPs (biosynthesized from DLLAE), when increased in concentration from lower dose (10 \ensuremath{\mu}g/mL) to higher dose (100 \ensuremath{\mu}g/mL), leads to an increase in antimicrobial response. Also, in future, this method can be employed in drug delivery system attributed to its cost which is economical when compared with other conventional approaches \unskip~\citep{692917:16400083}.
    
\section{Conclusion }
Current study was aimed to biosynthesize and determine the antimicrobial potential of SNPs of DLLAE. In this study, the SNPs were synthesized in eco-friendly way without using hazardous chemicals. The visual examination of color change to brown, UV-Vis and FTIR data confirmed the success of SNPs biosynthesis using DLLAE. The FESEM, EDX, and XRD data established the morphology of biosynthesized SNPs. The SNPs formed were poly dispersed and spherical in shape. The antimicrobial activity of SNPs formulated in present study establish that small sized SNPs (biosynthesized from DLLAE) when increased in concentration from low to high dose causes rise in antimicrobial response.  Hence, present study concludes that silver nanoparticles obtained from DLLAE strong response against \textit{B. subtilis, E. coli,} \textit{S. aureus,} and \textit{P. aeruginosa. } Study recommends DLLAE as potential resource to produce the potent antimicrobial SNPs. 
\section*{Acknowledgement}Authors acknowledge the facilities provided by AIMST University to accomplish this study. Extended thanks to NOR Lab, Universiti Sains Malaysia to assist in generation of spectral data.
    

\bibliographystyle{pharmascope_apa-custom}

\bibliography{\jobname}
\end{document}
